- Home
## Documents

*Eigenvalue buckling analysis of cracked functionally ...imechanica.org/files/2016-Eigenvalue...*

of 39/39

Accepted Manuscript Eigenvalue buckling analysis of cracked functionally graded cylindrical shells in the framework of the extended finite element method Amir Nasirmanesh, Soheil Mohammadi PII: S0263-8223(16)30970-9 DOI: http://dx.doi.org/10.1016/j.compstruct.2016.09.065 Reference: COST 7791 To appear in: Composite Structures Received Date: 19 June 2016 Revised Date: 17 September 2016 Accepted Date: 22 September 2016 Please cite this article as: Nasirmanesh, A., Mohammadi, S., Eigenvalue buckling analysis of cracked functionally graded cylindrical shells in the framework of the extended finite element method, Composite Structures (2016), doi: http://dx.doi.org/10.1016/j.compstruct.2016.09.065 This is a PDF file of an unedited manuscript that has been accepted for publication. As a service to our customers we are providing this early version of the manuscript. The manuscript will undergo copyediting, typesetting, and review of the resulting proof before it is published in its final form. Please note that during the production process errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain.

View

241Download

3

Embed Size (px)

Accepted Manuscript

Eigenvalue buckling analysis of cracked functionally graded cylindrical shellsin the framework of the extended finite element method

Amir Nasirmanesh, Soheil Mohammadi

PII: S0263-8223(16)30970-9DOI: http://dx.doi.org/10.1016/j.compstruct.2016.09.065Reference: COST 7791

To appear in: Composite Structures

Received Date: 19 June 2016Revised Date: 17 September 2016Accepted Date: 22 September 2016

Please cite this article as: Nasirmanesh, A., Mohammadi, S., Eigenvalue buckling analysis of cracked functionallygraded cylindrical shells in the framework of the extended finite element method, Composite Structures (2016), doi:http://dx.doi.org/10.1016/j.compstruct.2016.09.065

This is a PDF file of an unedited manuscript that has been accepted for publication. As a service to our customerswe are providing this early version of the manuscript. The manuscript will undergo copyediting, typesetting, andreview of the resulting proof before it is published in its final form. Please note that during the production processerrors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain.

http://dx.doi.org/10.1016/j.compstruct.2016.09.065http://dx.doi.org/10.1016/j.compstruct.2016.09.065

1

Eigenvalue buckling analysis of cracked functionally graded cylindrical shells in the

framework of the extended finite element method

Amir Nasirmanesh, Soheil Mohammadi

High Performance Computing Lab, School of Civil Engineering,

University of Tehran, Tehran, Iran.

ABSTRACT

In this study, eigenvalue buckling analysis for cracked functionally graded cylindrical shells

is performed using eight noded degenerated shell elements in the framework of the extended

finite element method. First, validity and efficiency of the proposed method in comparison

with available results are examined and then the approach is utilized for examining cracked

FGM cylindrical shells subjected to different loading conditions, including axial

compression, axial tension and combined internal pressure and axial compression. Also, the

effects of various parameters such as crack length and angle, gradient index of the material,

aspect ratio of the cylinder and internal pressure on the buckling behavior are extensively

investigated.

Keywords: Buckling, cylindrical shell, Extended finite element method (XFEM), Crack,

Functionally graded material (FGM)

Corresponding author, Address: High Performance Computing Lab, School of Civil Engineering, University of

Tehran, Tehran, Iran. Tel.: +98 21 6111 2258; fax: +98 21 6640 3808. E-mail address: [email protected]

2

1. Introduction

Composite shell structures have been extensively utilized for a broad range of applications

including space crafts, airplane fuselage, thermal coating barriers, defense systems and many

others due to their considerably high strength to weight ratio. Nevertheless, fiber reinforced

laminate shells suffer from many disadvantages such as delamination vulnerability to impact

loading, low resistance to sustain in thermal environments. Functionally graded materials are

a new class of composite materials which have obviated the interface-related problems in

traditionally laminate composites due to their continuous and smooth variation of materials

across the thickness. Usually, these materials consist of a ceramic surface, which can be

imposed to a high gradient of thermal loading, gradually changed into a metallic surface on

the other side to withstand in mechanical loadings. As a result, functionally graded

cylindrical shells have drawn special attention from the application and theoretical points of

view. Despite their superior characteristics, there are several failure modes which may

endanger the overall safety of these structures. Among them, buckling can be one of the

dominant failure modes. On the other hand, because functionally graded materials are often

used in extreme environments, they are highly prone to imperfections such as voids and

cracks in their structure during the production and life service. Hence, it is vital to perform

accurate buckling analyses for cracked functionally graded cylindrical shells to allow for

better and more reliable designs.

Many comprehensive studies have been performed on the buckling behavior of functionally

graded cylindrical shells in the past decade. Ng et al. [1] presented an analytical formulation

for dynamic buckling behavior of FGM cylindrical shells subjected to periodic loadings.

They found out that the gradient index of the material could crucially affect the buckling

behavior of the problem. Another analytical solution was presented by Sofiyev [2]

concerning the buckling analysis of FGM cylindrical shells subjected to axial dynamic

loadings. Further analytical studies for buckling and postbuckling of functionally graded

cylindrical shells can be found in [3-10].

On the other hand, there are only limited works on the buckling of cracked cylindrical shells.

Esteknachi and Vafai [11] studied the buckling behavior of isotropic cracked cylindrical

shells subjected to axial loading using the classical finite element method. They used a mesh

zooming scheme for adaptive generation of the mesh of the cylindrical shell so that with

approaching to the crack tip the size of the elements would decrease from the standard size of

the uncracked regions to a very finer size to better capture the crack tip stress singularity.

They also performed a similar study for cracked plates [12]. The effect of internal pressure on

the buckling behavior of cracked cylindrical shells subjected to combined internal pressure

and axial compression was investigated by Vaziri and Estekanchi [13] using the commercial

FEM package ANSYS. They concluded that the effect of the internal pressure on the

buckling stresses became completely different depending on the crack being axial or

circumferential. For instance, when the crack was in the axial direction of the cylinder, the

internal pressure had a detrimental effect on the buckling stresses, whereas, for the

circumferential crack, the internal pressure had a stabilizing effect on the buckling behavior

[13]. Also, Vaziri [14] carried out a linear eigenvalue buckling analysis using the finite

3

element method to study the effect of crack length, crack orientation and the sequence of the

lamina on the buckling behavior of composite cylindrical shells under axial compression.

Dynamic stability and vibration of cracked cylindrical shells under compressive and tensile

periodic loadings were investigated using the finite element method by Javidruzi et al. [15].

They showed that the existence of crack could considerably decrease the natural frequency of

the shell. Also, Tafreshi [16-18] performed a series of delamination buckling and

postbuckling analysis for laminate composite cylindrical shells under various loading

conditions by the finite element method.

In addition, there are a few works which have addressed the buckling analysis of cracked

plates in the framework of the extended finite element method. Recently, Nasirmanesh and

Mohammadi [19] performed an eigenvalue buckling analysis for cracked composite plates

using the extended finite element method. They examined several problems and thoroughly

investigated the effects of different parameters such as crack lengths, crack angles and

direction of fibers on the buckling behavior of composite plates. They also concluded that

even for the tensile loading, changes in the fiber direction can alter the local instability

around the crack faces to a global buckling mode.

Natarajan et al. [20] carried out thermo-mechanical buckling analysis of cracked functionally

graded plates in the framework of the partition of unity method and examined the effects of

gradient index of the material and crack lengths on the critical temperature and critical

buckling stresses. Another XFEM buckling analysis for cracked FGM rectangular plates

subjected to compressive loading was reported by Liu et al. [21]. Baiz et al. [22] used the

smooth curvature method to study the effects of crack lengths and locations on the critical

buckling stresses for isotropic plates. None of the existing works have studied the buckling

behavior of cracked functionally graded shells. The novelty of the present study is, for the

first time, to propose an XFEM shell formulation to carry out an eigenvalue buckling analysis

for cracked FGM cylindrical shells.

XFEM was motivated by disadvantages of the classical finite element method for fracture

analysis; including the need for mesh conformity to crack path and incapability to capture the

exact stress field near a crack tip. In XFEM, while cracks are represented independent of the

mesh, the exact analytical stress field around the crack tip is achieved. The method has been

extended to static and dynamic orthotropic problems for both fixed and propagating cracks

[23-30], bi-materials [31, 32] and FGMs [33]. Recently, Rashetnia and Mohammadi [34]

proposed a new set of tip enrichment functions for studying the fracture behavior of rubber-

like materials which experience large deformations. They concluded that the logarithmic set

of enrichment functions are more accurate and efficient.

There are other approaches that are capable of handling complex problems including

nonlinear dynamic fracture and fluid driven fracture of plates and shells. For instance,

Nguyen-Thanh et al. [35] proposed a model based upon the extended isogeometric method in

accordance with the Kirchhoff-Love theory to analyze thin shells. In addition, a meshfree

method was proposed for nonlinear dynamic fracture analysis of thin shells, which allowed to

predict crack propagation across the thickness of shell [36, 37]. Recently, the phase-field

4

method has been utilized to study the fracturing behavior of plates and shells [38, 39] with

the goal of avoiding explicit track of cracks in special problems.

The present paper is organized as follows: the basic formulation of the functionally graded

problem is presented. Definition of degenerated shell elements is followed by deriving the

stability equations in the framework of the extended finite element method. Numerical

simulations are presented and discussed for verifying the proposed method and then extended

to cracked FGM problems in Section 3. Finally, a brief review of the concluding remarks is

presented.

2. Theoretical formulation and XFEM discretization

In this study, the Youngs module (zE ) of the problem is assumed to vary across the

thickness; from the pure metallic surface at the bottom (mE ) to the fully ceramic surface at

the top (cE ) of the shell based on a power distribution law,

m c m

1( )

2

n

z

zE E E E

t

= + +

(1)

where t is the thickness of shell, n is the gradient index of the material and z changes along

the thickness so that 2 2t z t , as shown in Fig.1. The Poissons ratio , however, is

assumed constant.

c

s

s

te

5

Fig. 1. Geometry of the cracked cylindrical shell and variation of material properties across

the thickness

In order to avoid mesh distortion and shear locking that usually occur in buckling

phenomena, 8-noded shell elements are adopted to discretize the domain [19, 40]. Geometry

of the shell is defined using the coordinates of the mid-surface of the shell and the unit

normal vector, which is perpendicular to the surface of the shell at each node, 3i

V , as

depicted in Fig. 2,

{ }8 8

3

1 1

; , ,2

Ti i

i i i i

i i

tN N x y z

= =

= + = x x V x (2)

Fig. 2. Eight noded shell element and local unit vectors.

where, i

N s are the shape functions of the plane eight noded element, i

t is the thickness of

the shell at each node (which is assumed constant in all nodes in this study) and of the

natural coordinate system is perpendicular to the surface of the shell at each node.

Consider a cracked FGM medium, depicted in Fig. (3), the displacement field of the problem

in the framework of the extended finite element method is presented as

FE Enr

u

v

w

= = +

u u u

(3)

6

xy

r

Crac

k

Fig. 3. Cracked medium and local crack tip coordinates.

where, , and wu v are the displacement components in the global coordinate , andx y z

directions, respectively. FE

u and Enr

u are the conventional continuous finite element

approximation and the approximation of the discontinuous part of the displacements,

respectively. FE

u can be written as,

1 18 8

FE 2 2

1 1

2 3

2

i i

i y x

i iii i i i y i x

i i i i

i y x

u e et

N v N e e

w e e

= =

= +

u

(4)

where andi iyk xk

e e are the components of the unit orthonormal vectors of the unit normal

vector at node i , i.e. 3i

V . andi i

are the rotational degrees of freedom with respect to

and yx axes, respectively.

Enru is composed of two separate parts to account for discontinuous and singular fields; each

part enriches the displacement field with specific enrichment functions to overcome the

limitation of the conventional finite element method. As a result, neither the mesh conformity

to the crack edges nor the mesh refinement around the crack tip is required.

Enr Heaviside Tip= +u u u (5)

( ) ( )1 1 18 8

Heaviside 2 2 2

1 1

3 2 3

2

i i i

y x

i i i i iii i y x

i ii i i

y x

a e et

N H a N H a e a e

a e e

= =

= +

u x x

(6)

7

( ) ( )( ) ( ) ( )( )

( ) ( )( )

18 4 8 1

Tip 2

1 1 1 1

3

1 18 4

2 2

1 1

2 2

0

0

0

2

i

i

i j j j i j j j

i j i j i

i i

y x

i i i iii j j j j y j x

i j i i

y x

b

N F F b N G G

b

e et

N R R b e b e

e e

= = = =

= =

= + +

+

u x x x x

x x

(7)

where, and bi ij j

a are the additional enrichment degrees of freedom. The vector of nodal

displacements ( d ) and enrichments ( andh t ) are defined as

{ }, , , ,T

u v w =d (8)

{ }1 2 3, , , ,T

a a a a a =h (9)

{ }1 2 3, , , ,T

b b b b b =t (10)

and the vector of unknowns D ,

{ }1 2 3 4T

=D d h t t t t (11)

In Eq. (6), ( )H x is the Heaviside function and is defined as [41]

1 above thecrack( )

1 under thecrackH

+=

xx

x

(12)

Also, the in-plane, out of plane and rotational enrichment functions in the local polar

coordinate system ( ,r ) are expressed as [40],

( ) ( ) ( ), sin , cos , sin sin , cos sin2 2 2 2

F r r r r r

=

(13)

( , ) sin2

G r r

=

(14)

( ) ( ) ( ), sin , cos , sin sin , cos sin2 2 2 2

R r r r r r

=

(15)

To obtain the governing equations, the total potential energy is written as:

8

b = + (16)

where b

is the bending strain energy and represents the membrane energy, necessary in

buckling problems [42] and is the potential of external loads.

1

2

T

b L Lv

dV = C (17)

0

T

NLv

dV = (18)

T

vdV = u q

(19)

where 0

is the tensor of initial stresses, which is computed from a static analysis, C is the

matrix of the material property, q is the traction tensor, and L & NL are the linear and

nonlinear terms of the Green-Lagrange strains, respectively,

, , , , ,

T

L

u v w v u w v u w

x y z x y y z z x

= + + +

(20)

2 2 2

2 2 2

2 2 2

1 1 1

2 2 2

1 1 1

2 2 2

1 1 1

2 2 2NL

u v w

x x x

u v w

y y y

u v w

z z z

u u v v w w

x y x y x y

u u v v w w

y z y z y z

u u v v w

z x z x

+ +

+ +

+ +

=

+ +

+ +

+ +

w

z x

(21)

{ }0 0 0 0 0 0 0, , , , ,T

x y z xy yz xz = (22)

Also, strain and stress tensors are related by the tensor of material properties C ,

= C (23)

9

11 12 12

12 11 12

12 12 11

44

44

44

0 0 0

0 0 0

0 0 0

0 0 0 0 0

0 0 0 0 0

0 0 0 0 0

C C C

C C C

C C C

C

C

C

=

C

(24)

where ij

C components depend only to the modulus of elasticityz

E and the Poissons ratio

of the material,

( )11 12 442 2, ,

1 1 2 1

z z zE E EC C C

= = =

+

(25)

Eq. (18) can be rewritten as:

{ }0 , ,y ,z , , , , , ,1

where2

TT

x x y z x y zv

dV = = S u u u v v v w w w (26)

0S is computed from the stresses obtained from the first stage of the buckling analysis; a

static analysis,

0 0 00

0 0 0

0 0 0

0 0 0

0

;

x xy xz

xy y yz

xz yz z

= =

S 0 0

S 0 S 0 S

0 0 S

(27)

Vectors of , andL

u are related to the nodal displacement vector D as

, = andL G

= =BD B D u ND (28)

where andG

B B correspond to linear and nonlinear parts of the Green-Lagrange strain,

respectively [19], and N is constructed from the shape functions as

1 1

/

2 2

3 3

0 02 2

0 02 2

0 02 2

i ii x i y i

r s i ii i x i y i

i ii x i y i

t te e

t te e

t te e

=

N

(29)

Substituting Eq. (28) into Eqs. (17), (18) and (19), the total potential energy becomes

0

1 1

2 2

T TT T T

G GV V V

dV dV dV = + D B CBD D B S B D D q (30)

10

Based on the principle of minimum potential energy, variation of the total potential energy

must vanish at equilibrium ( 0 = ),

( ){ }0 0 0T T TG GV V V

dV dV dV = + = D B CB B S B D N q D (31)

Applying the XFEM displacement approximation (3), the following equilibrium state is

obtained after some manipulation and simplification [42]

ext{ }{ }+ =

GK K D F (32)

where K and GK are the conventional and geometric stiffness matrices, respectively, and

extF is the vector of external forces.

For a linear problem, if the external load vector is multiplied by a factor , then, the

geometric stiffness matrix is also multiplied by ,

ext{ }{ } + =

GK K D F (33)

Having the definition of buckling by Cook [42], when buckling occurs, the external load does

not change for an infinitesimal displacement of dD ,

ext{ }{ }d + + =

GK K D D F (34)

Subtracting Eq. (34) from Eq. (35) leads to the stability equation of the problem,

{ }{d } 0+ =G

K K D (35)

where is the eigenvalue of the system. The buckling stress is obtained by multiplying to

the initial external stress of the system, and the minimum value of corresponds to the

critical buckling stress of the system. For any specified value of , there is an eigenvector

dD which represents the buckling mode shape of the problem.

( ) ( )rs r T sij i j

vdV= K B C B (36)

0( ) ( ) ( , , , )rs r T s

G ij G i G jv

dV r s= =K B S B d h t (37)

( )extT

rs rs

i iV

dV= F N q (38)

For facilitating the construction of / / /, andr s r s r si Gi i

B B N for different , , ,r s = d h t , the

following functions are defined

( ) ( )( )i j j iN F F = x x

11

( ) ( )( )i j j iN R R = x x (39)

( ) ( )( )i j j iN G G = x x

So

, 1 1

, ,x

, 2 2

, ,

, 3 3

, ,

1 1

, ,

, ,

/

2 2

,

0 02 2

0 02 2

0 02 2

2 20

2 2

i ii x x i y i

x

i ii y x i y i

y y

i ii z x i y i

z z

i ix i y i

y y

i y i x

r s i ix i yi

x

t te e

t te e

t te e

t te e

t te e

+ +

=

B,

2 2

, ,

, ,

3 3

, ,

1 1

, ,

, ,

3 3

, ,

2 20

2 2

2 20

2 2

i

x

i ix i y i

z z

i z i y

i i

x i y i

y y

i ix i y i

z z

i z i x

i i

x i y i

x x

t te e

t te e

t te e

t te e

+ +

+ +

(40)

12

, 1 1

, ,

, 1 1

, ,

, 1 1

, ,

, 2 2

, ,

/, 2

,

0 02 2

0 02 2

0 02 2

0 02 2

0 02 2

i ii x x i y i

x x

i ii y x i y i

y y

i ii z x i y i

z z

i ii x x i y i

x x

i ir si y x iGi

y

t te e

t te e

t te e

t te e

t te e

=

B 2,

, 2 2

, ,

, 3 3

, ,

, 3 3

, ,

, 3 3

, ,

0 02 2

0 02 2

0 02 2

0 02 2

y i

y

i ii z x i y i

z z

i i

i x x i y i

x x

i ii y x i y i

y y

i i

i z x i y i

z z

t te e

t te e

t te e

t te e

(41)

( )

: /

: / ( ) H( )

: / , , as defined in equation (33)

i

i i

if r s N

if r s N H

if r s

= = = =

= = = =

= =

d

h x x

t

(42)

It should be noted that because of the highly complex stress field around the crack tip and the

displacement discontinuity across the crack faces, the conventional Gauss quadrature

integration technique is not adequate to properly evaluate the integrals of Eqs. (36), (37) and

(38). In this study, the sub-triangulation method along with the Gauss quadrature rule is

adopted due to its simplicity and acceptable accuracy [21-23]. In this approach, 13 Gauss

points per triangle are considered for elements enriched by the tip enrichment functions,

while, for split elements, 7 Gauss points are adopted per triangle, and a simple 2 2 Gauss

quadrature rule is used for the standard ordinary elements, as depicted in Fig. 3.

13

Fig. 3. Element types and their associated enriched nodes, triangulation and Gauss points

2. Numerical simulations

In this section, linear eigenvalue buckling analysis is performed for several mixed-mode

cracked homogeneous and inhomogeneous FGM plates and cylindrical shells in the

framework of the extended finite element method. Due to the fact that there is no published

document on the buckling of cracked functionally graded cylindrical shells, first, a problem

of cracked FGM plate under compressive loading is analyzed to show the capability of the

proposed method and to perform the required comparisons. Then, buckling of a cracked

isotropic cylindrical shell under combined internal pressure and compressive loading as well

as pure axial tension is investigated and the obtained results are verified with available

studies. Afterward, a perfect functionally graded cylindrical shell subjected to axial

compression is adopted and the predicted buckling stresses are compared with the available

results. A thorough study is then carried out on the buckling behavior of mixed-mode cracked

functionally graded cylindrical shells subjected to three different cases of loading including

axial tension, axial compression and combined internal pressure and axial compression. In

addition, the effect of different parameters such as crack lengths, crack angles, gradient index

of the material, thickness and the aspect ratios of the shell on the buckling behavior are

extensively discussed. Finally, because the proposed XFEM approach can handle the

problems with multiple cracks without any additional complexity, the buckling analysis is

performed on a compressive FGM cylindrical shell with three parallel cracks.

2.1. Cracked FGM rectangular plate subjected to uniaxial compressive loading

14

As the first example, a central cracked FGM rectangular plate under compression, as depicted

in Fig. 4, is considered. It is assumed that the elasticity modulus of the plate varies through

the thickness based on a power distribution law, from the fully metallic surface in the bottom

to the fully ceramic in the top surface of the plate. This problem has recently been studied by

a so-called stabilized discrete shear gap extended 3-node triangular plate element [21]. The

youngs modulus is 9m 70 10 MPaE = and

9

c 151 10 MPaE = on metallic and ceramic

surfaces, respectively. Also, the constant Poissons ratio of 0.3 is assumed through the

thickness.

A 35 35 structured mesh is adopted for the eigenvalue buckling analysis and the computed

critical buckling stresses are normalized by the parameter 2 0 2 2 3uni c12(1 ) x crk b t E = .

The aspect ratio of the plate, thickness, crack length and the angle of the crack are adopted as

/ 1a b = , / 0.01t a = , / 0.6c a = and 0 = , respectively.

Fig. 4. A central cracked FGM plate under compression

Computed normalized buckling parameters for different values of gradient index of the

material are shown in Table 1. It is observed that the buckling stress decreases as the gradient

index of the material increases. Also, very close results to reference [21] are obtained;

showing sufficient accuracy for modeling the buckling behavior of cracked functionally

graded plates.

15

Table 1. Normalized buckling parameters of a central cracked FGM plate for various values

of gradient indices of material ( n )

n unik

Ref [21] Present study Difference (%)

0.0 2.9995 3.0148 0.51

0.2 2.6548 2.6760 0.80

0.5 2.3470 2.3552 0.35

1.0 2.0977 2.1166 0.90

2.0 1.9222 1.9262 0.21

5.0 1.7825 1.7860 0.20

10.0 1.6751 1.6828 0.46

2.2. Cracked homogeneous cylindrical shells

2.2.1. Simultaneous internal pressure and axial compression

As the second example, the problem of buckling of a cracked homogeneous isotropic

cylindrical shell for two different loading conditions; including combined internal pressure

and axial compression and pure axial tension, is considered. This problem was earlier

investigated comprehensively by Vaziri and Estekanchi [13] and Seifi et al. [43] using

commercial finite element analysis programs. Very fine meshes were adopted to model the

stress concentration at the crack tips. In the present study, the stress singularity at crack tips is

captured in a more accurate manner using the tip enrichment functions. Then, the bifurcation

buckling analysis is performed in the framework of the extended finite element method.

First, the same problem of [13] is considered (Fig. 1). Material and geometric properties of

the problem are 69 GPaE = , 0.3 = , 2 mL = , 0.5mR = and 0.5mmt = . Here, only a

comparison is made between the results of the present XFEM and the classical finite element

method to assess the reliability of the proposed method for modeling this complex instability

problem.

A dimensionless buckling load factor is defined as the ratio of the computed critical

buckling stress of the cracked cylindrical shell ( cr ) to the theoretical buckling stress of the

perfect cylindrical shell subjected to axial compression ( th ),

16

cr

th

=

(43)

th23(1 )

E t

R

=

(44)

Also, another dimensionless loading parameter is defined as the ratio of the induced

membrane stress due to internal pressure ( membrane ) to the total axial compressive stress,

developed due to internal pressure and axial compression ( axial ), in the perfect cylindrical

shell.

membrane

axial

=

(45)

membrane

pR

t =

(46)

where p is the internal pressure applied on the inner surface of the cylinder.

First, an un-cracked cylindrical shell is considered and the effect of the internal pressure on

the buckling stress associated with the first buckling mode is examined. It can be observed

from Fig. 5 that with increasing the internal pressure the buckling stress increases slightly,

which is consistent with the available results [13].

0 10 20 30 40 50 60 70 80 901

1.001

1.002

1.003

1.004

1.005

1.006

1.007

Dimensionless loading parameter,

Dim

ensi

on

less

bu

ckli

ng

lo

ad,

Mode I Present study

Mode I Ref [13]

17

Fig. 5. Effect of the internal pressure on the buckling stress of the first buckling mode for the

un-cracked cylindrical shell

Then, an axially cracked cylindrical shell subjected to combined internal pressure and axial

compression is considered and the critical buckling stresses are obtained for various internal

pressures by the present method and then compared with available reference results [13], as

plotted in Fig. 6. It is observed that, the computed buckling load parameters ( ) are in the

very good agreement with the reference results [13]. It should be noted that, the number of

elements was not mentioned in Ref [13], so it is not possible to further compare the efficiency

of the two methods. Moreover, it is observed that, for small crack length ratios ( / R 0.05a = ),

with increasing the internal pressure, the buckling load parameter starts to increase, followed

by a decreasing trend, showing the stabilizing effect of the internal pressure at low values. On

contrary, for larger crack length ratios ( / R 0.1a = ), the internal pressure has a destabilizing

effect on the buckling behavior of the cylinder, because with increasing the internal pressure,

the buckling stress decreases.

[13]

[13]

Fig. 6. Buckling load parameters versus internal pressure for axially cracked cylindrical shell

To further examine the efficiency of the present XFEM formulation, a circumferentially

cracked cylindrical shell ( 0 = ) subjected to combined internal pressure and axial

compression [13] is considered. Variations of the computed buckling load parameter versus

the internal pressure are compared with reference [13] in Fig. 7, which shows a good

agreement. In contrast to the case of axial crack ( 90 = ), the internal pressure improves the

local buckling behavior of cylinder due to its stabilizing effect on crack faces. Also, it is

18

observed that for relatively long cracks, the effect of internal pressure is more significant on

the buckling behavior of the cylindrical shell (Fig. 7).

0 5 10 150.4

0.5

0.6

0.7

0.8

0.9

1

1.1

Dimensionless loadin Parameter,

Dim

ensi

onle

ss b

uck

ling l

oad

,

a/R=0.20Ref

a/R=0.15Ref

a/R=0.20XFEM

a/R=0.15XFEM

Fig. 7. Buckling load parameters versus internal pressure for circumferential cracked

cylindrical shell

2.2.2. Pure axial tensile load

A simply supported cracked cylindrical shell subjected to axial tension, recently studied by Seifi et al. [43], is considered. The material properties are 70 GPaE = and 0.3 = , and the

geometric specifications are 300 mmL = , 60 mmR = , 1.5mmt = , 45 = and / 1.0a R = . A

structured 35 45 (35 elements in the circumferential and 45 elements in the longitudinal direction) mesh is adopted for the analysis.

The critical buckling stress related to the first mode of buckling is predicted as

231.9 MPacr

= , which is in good agreement with the reference value of 231.81MPa = .

Reference [43] used 3466 elements with 5 Gauss integration points in the thickness direction

that leads to the total number of 17330 Gauss points, which is far more than the total number of Gauss points and elements used in this study, since only two Gauss integration points

considered across the thickness (1575 elements and 3150 Gauss points). The ability of the present method to capture the stress singularity at crack tips without refining the element size

allows for higher accuracy and lower computational cost than the reference finite element

solution [43], i.e. the approach employed for this particular case results in 5.5 times less

computational cost.

19

2.3. Functionally graded cylindrical shells

After examining the accuracy and efficiency of the proposed XFEM in handling the problem of buckling of cracked homogeneous cylindrical shells, the method is now applied for

modeling the more complex problem of buckling analysis of cracked functionally graded shells.

First, the problem of buckling analysis of an un-cracked FGM cylindrical shell under

compressive load is considered and the validity of the proposed method is verified with

available reference [44]. Then, the method is adopted for buckling analysis of cracked

functionally graded cylindrical shells for three different cases of loading conditions; axial

tension, axial compression and combined internal pressure and axial compression, as well as

a compressive FGM cylindrical shell with three parallel cracks.

2.3.1. Uncracked FGM cylindrical shell subjected to axial compression

Consider a simply supported functionally graded cylindrical shell, which is subjected to axial

compression, as depicted in Fig. 1. The length to the radius ratio of the shell is / 2L R = and

the effects of different radius to thickness ratios ( /R t ) and gradient index of the material ( n

) on the buckling behavior are investigated by the present method and compared with the

available reference results [44]. The material properties of the problem are 5 4

c m3.8 10 MPa and 7 10 MPaE E= = on the ceramic and metallic sides of the FGM

thickness, respectively, and the Poissons ratio is considered constant across the thickness (

0.3 = ).

Computed buckling stresses for various gradient indices are normalized by cE and then

plotted versus different radius to thickness ratios of the cylinder in Fig. 8. Clearly, the

obtained results are very close to the reference results [44]. In addition, as the gradient index

increases, the normalized buckling stress decreases significantly. Moreover, increasing the

radius to thickness ratio affects the buckling behavior of the cylinder dramatically.

20

100 200 300 400 500 600 700 800 900 10000

10

20

30

40

50

60

R/t

No

rma

lize

d b

ucklin

g s

tre

ss

n=0.1Present study

n=0.1Ref [39]

n=2.0Present study

n=2.0Ref [39]

Fig. 8. Normalized buckling stress against the radius to thickness ratio for an uncracked FGM

cylindrical shell subjected to axial compression

2.3.2. Cracked FGM cylindrical shell subjected to axial tension

In this section, the buckling analysis is carried out using the proposed XFEM method for

extracting the critical buckling stress of a simply supported mixed-mode cracked functionally

graded cylindrical shell under axial tension, as shown in Fig. 1. It should be noted that, under

a uniform axial tensile load, a cracked cylindrical shell can buckle locally around the crack

faces due to the generated compressive stress fields in these region. The material properties

of the thin cylindrical shell is assumed similar to Section 2.3.1 and the length to radius ratio (

/L R ) and the radius to thickness ratio ( /R t ) of the shell are 4 and 1000, respectively.

All cracked FGM shells are modelled by a 45 55 structured mesh (45 elements in the

longitudinal and 55 elements in the circumferential direction), unless otherwise mentioned.

The effects of crack lengths and angles, gradient index of material, thickness and the length

of the cylinder on the buckling behavior of the shell are investigated comprehensively. Also,

the buckling mode shapes are presented to better illustrate the local instability of crack edges.

The tensile buckling stresses for different crack lengths and gradient indices for crack

direction of 0 = are presented in Table 2. It is observed that the predicted critical buckling

stresses are so sensitive to the ratio of the crack length to radius of the shell, so that for the

constant gradient index 2n = , the buckling stress dramatically decreases from 1675MPa to

148 MPa when the ratio of the crack length to radius increases from 0.5 to 1.0. Furthermore,

with increasing the gradient index of the material, the expected buckling stress decreases. For

21

example, when the crack length to radius ratio is equal to 1.0 and the gradient index is

0.5n = , the buckling stress is approximately two times higher than its value for 10n = .

Table 2. Critical buckling stresses for various gradient indices and crack length to radius

ratios for a circumferentially cracked FGM cylindrical shell subjected to axial tension

/a R n

0.5 1 2 4 6 10

Critical buckling Stress (MPa)

0.5 2717 2165 1675 1336 1194 1054

0.7 1397 1099 853 700 638 572

1.0 243 191 148 122 112 101

1.2 172 136 105 86 78 69

For examining the effects of crack orientation on the buckling behavior of the problem, Fig. 9

compares the results for various crack angles for the constant gradient index of 2.0n = .

Clearly, with increasing the crack angle, the buckling stress increases significantly. For

instance, for the case of / 1.0a R = , the critical buckling stress for 60 = is approximately 7

times greater than the buckling stress for 0 = .

0 10 20 30 40 50 600

200

400

600

800

1000

1200

Crack angle (Degree)

Ten

sile

buck

ling s

tres

s (M

Pa)

a/R=1.0

a/R=1.2

a/R=1.5

Fig. 9. Tensile buckling stresses for different crack angles for a FGM cylindrical shell

22

Fig. 10 examines the effects of thickness and length of the cylinder on the critical buckling

stress. The results are related to the case of 4.0n = and / 1.0a R = . Accordingly, the length

to radius ratio of the cylinder highly affects the buckling behavior so that with decreasing the

length to radius ratio the buckling stress significantly decreases. For instance, the buckling

stress for the case of / 2.0L R = and / 400R t = is approximately 3.4 times greater than the

case with the same thickness and / 0.5L R = . Clearly, the buckling stress is so sensitive to

the radius to thickness ratios, where increasing the radius to thickness ratio leads to a

considerable reduction in the buckling stress.

400 450 500 550 600 650 700 750 800 850 90020

40

60

80

100

120

140

160

180

200

R/t

Ten

sile

bu

ckli

ng

str

ess

(MP

a)

L/R=0.5

L/R=1.0

L/R=2.0

Fig. 10. Effect of the aspect ratio of the cracked FGM cylindrical shell on the critical tensile

buckling stress

The buckling mode shapes related to the case of gradient index 2n = and / 1.2a R = are

presented in Fig. 11. The local instability of crack edges are clearly observed in the Fig. 11.

Higher critical stresses are obtained for the second and third modes of buckling.

23

Fig. 11. The first three buckling mode shapes of the circumferentially cracked FGM

cylindrical shell subjected to axial tension

24

Moreover, in order to investigate the sensitivity of the results to the number of elements,

different number of meshes are adopted for the case of / 0.5a R = and 6.0n = and the

buckling stresses are obtained. It is observed from the Fig. 12 that by increasing the number

of elements, the buckling stress converges to 1197.63MPa .

500 1000 1500 2000 2500 3000 3500 4000 4500 5000500

600

700

800

900

1000

1100

1200

1300

Number of elements

Tensile

bucklin

g s

tress (

MP

a)

Fig. 12. Sensitivity of the buckling stress to the number of elements for the circumferential

cracked FGM cylindrical shell subjected to axial tension

It is clearly demonstrated that cracked functionally graded cylindrical shells, even in the

tensile loading condition, which is the safest loading state, are highly prone to local buckling

around the crack faces. Moreover, even a slight increase in the crack length could

substantially jeopardize the stability of the cylinder.

2.3.3 Cracked functionally graded cylindrical shell subjected to axial compression

Buckling analysis for cracked functionally graded cylindrical shell subjected to axial

compression in general mixed-mode condition is now performed with the developed

extended finite element method. Geometric parameters and material properties of the shell

are similar to Section 2.3.2, unless mentioned otherwise. Besides, it is investigated that how

different parameters such as crack lengths and orientations, gradient index of the material,

thickness and the length of the shell can influence the buckling behavior of the FGM

cylindrical shell.

First, the effects of crack length to radius ratio ( / Ra ) and the gradient index of the material

on an axially cracked ( 90 = ) FGM shell are examined. According to Fig.13, different

conclusions can be made. First, the crack length substantially affects the buckling behavior of

the shell. For example, for the constant gradient index 0.5n = , the buckling stress related to

25

/ 1.0a R = is decreased significantly from 43.35 MPa to 24.72 MPa , associated with the

crack length to radius ratio of / 2.5a R = . Then, the buckling stress can crucially be affected

by the gradient index of the material, so higher increase of the gradient index leads to more

reduction in the buckling stress. Also, it can be noted that for all cases of crack lengths, the

buckling stresses for 0.5n = are approximately 2.6 times greater than those in which 10n = .

1 2 3 4 5 6 7 8 9 100

5

10

15

20

25

30

35

40

45

Gradient index

Cir

itci

al b

uck

lin

g s

tres

s (M

Pa)

a/R=1.0

a/R=1.5

a/R=2.0

a/R=2.5

Fig. 13. Effects of the crack length ratios and the gradient index on the buckling stress of

axial cracked FGM cylindrical shell under axial compression

To better illustrate how the presence of crack can alter the buckling behavior of the FGM

cylindrical shell, the first four buckling mode shapes and their corresponding buckling

stresses for uncracked and axially cracked FGM cylindrical shells are presented in Fig. 14.

Clearly, existence of the crack can totally change the buckling behavior from the global

buckling to local buckling around the crack faces in a very lower value of critical applied

stress.

26

Fig. 14. The first four buckling mode shapes for (a) uncracked and (b) axially cracked

functionally graded cylindrical shell subjected to axial compression

27

In order to investigate the influence of crack orientation on the buckling behavior of the

problem, the critical compressive buckling stress for different crack lengths and orientations

for the constant gradient index 2.0n = are computed and depicted in Fig. 15. It is observed

that variations of crack lengths and angles lead to different and complex buckling behaviors,

making it impossible to make a general conclusion. Notwithstanding, for all /a R cases, the

minimum critical buckling stress corresponds to the axial crack ( 90 = ).

0 10 20 30 40 50 60 70 80 9010

20

30

40

50

60

70

80

90

Crack Angle (Degree)

Cri

tica

l buck

ling s

tres

s (M

Pa)

a/R=0.7

a/R=1.0

a/R=1.2

a/R=1.5

Fig. 15. Compressive buckling stresses for different crack lengths and angles

Fig. 16 is given to probe the effects of aspect ratios of shell on the critical buckling stresses

for / 0.8a R = , 4.0n = and 90 = . Generally, with increasing the radius to thickness ratios

(decreasing the thickness), the buckling stress decreases considerably. Nevertheless, the

critical buckling stresses are not highly affected by variation of the length of the cylinder. For

instance, for the case of / 400R t = , the buckling stress decreases about 15% when the length

to radius ratio of the cylinder decreases from 3 to 1.

28

400 450 500 550 600 650 700 750 800 850 90015

20

25

30

35

40

45

50

R/t

Com

pre

ssiv

e buck

ling s

tres

s (M

Pa)

L/R=1.0

L/R=2.0

L/R=3.0

Fig. 16. Effects of aspect ratios on the critical buckling stresses of the axially cracked FGM

cylindrical shell subjected to compression

Also, Fig. 17 presents the influence of crack orientation and length of the shell on the

buckling behavior. The first four buckling mode shapes and their associated buckling stresses

for two different cases of 15 and =30 = and the length to radius ratio of / 2L R = and

/ 50R t = are shown in Fig. 17. Based upon the plots given in Fig. 14 and Fig. 17, it is

observed that any variations in crack orientation or the geometrical parameters (

/ and /L R R t ) severely alter the buckling behavior of the cracked FGM cylindrical shell.

29

Fig. 17. The first four compressive buckling mode shapes for mixed-mode cracked FGM

cylindrical shell a) 15 = b) 30 =

30

2.3.4. Cracked functionally graded cylindrical shell subjected to combined internal

pressure and axial compression

One of the dominant loading conditions in the cylindrical shells is when simultaneous axial compression and internal pressure are applied to the shell. This problem with homogeneous

isotropic material was briefly studied in Section 2.2 and verified with the available results.

Now, the problem is further extended to cracked FGM cylindrical shell and the buckling

analysis is performed using the extended finite element method. The material properties and

geometric parameters are identical to previous FGM examples and the shell is simply

supported at the both ends.

Fig. 18 presents the effect of crack length to radius ratio and gradient index of the material on

the critical internal pressure which causes buckling. It is observed that the critical internal

pressure decreases significantly as the crack length ratios and gradient index increase.

0 1 2 3 4 5 6 7 8 9 100

0.001

0.002

0.003

0.004

0.005

0.006

0.007

0.008

0.009

0.01

Gradient Index

Cri

tica

l In

tern

al P

ress

ure

(M

Pa)

a/R=1.0

a/R=1.5

a/R=2.0

a/R=2.5

Fig. 18. Effects of gradient index and crack length ratios on the critical internal pressure for

the axially cracked FGM cylindrical shell subjected to internal pressure

Fig. 19 depicts the effects of internal pressure on the critical axial compressive buckling

stresses for axially cracked functionally graded cylindrical shell in terms of various crack

length to radius ratios for the constant value of 2.0n = . cP denotes the critical internal

pressure, computed in Fig. 18. It is observed that the internal pressure has a detrimental effect

on the buckling behavior, where, with increasing the applied internal pressure, the axial buckling stress decreases dramatically. Also, for high values of internal pressure, buckling

occurs at approximately the same axial compression for all crack lengths.

31

0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.81

2

3

4

5

6

7

8

9

P/Pc

Ax

ial

Bu

ckli

ng

Str

ess

(MP

a)

a/R=0.5

a/R=1.0

a/R=1.5

a/R=2.0

a/R=2.5

Fig. 19. Effect of internal pressure on the critical axial buckling stress for the axially cracked

FGM cylindrical shell for different values of crack length ratios and 2.0n =

Now, the effect of internal pressure on the circumferential cracked FGM cylindrical shell is

examined. According to Fig. 20, the critical buckling stress highly depends to the internal

pressure. Also, it should be noted that, in contrast to the axially cracked cylinder, the internal

pressure has a significant stabilizing effect on the buckling behavior of the circumferential

cracked functionally graded cylindrical shell.

32

0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8100

120

140

160

180

200

220

P/Pc

Ax

ial

bu

ckli

ng

str

ess

(MP

a)

a/R=0.5

a/R=0.7

a/R=1.0

Fig. 20. Effects of internal pressure on the critical buckling stresses for circumferential

cracked FGM cylindrical shell for different crack length ratios and 2.0n =

2.3.5 FGM cylindrical shell with multiple cracks subjected to axial compression

Compared with the conventional finite element method, one of the advantages of XFEM is its

ability to model problems involving multiple cracks without noticeably altering the geometry

of the mesh. Thereupon, as the last example, the buckling behavior of an FGM shell with

three parallel cracks subjected to compression, as depicted in Fig. 21, is investigated.

Geometric and material properties of the shell is identical to those in the previous examples.

Also, the shell is clamped at both ends. The effect of the distances between the cracks on the

critical buckling stress and the corresponding mode shapes are probed.

33

Clampededge

Clampededge

a

Fig. 21. An FGM cylindrical shell with three parallel cracks

For investigating the effects of crack length and distance between cracks, critical buckling

stresses associated with 2.0n = are obtained and presented in Table 3. Clearly, the buckling stresses are drastically decreased by increase of crack lengths. For instance, in the casse of

/ 0.05d L = , the buckling stress for / 1.5a R = is 6 times greater than the case associated with / 0.7a R = . Besides, the buckling behavior of shell is affected by the variation of distance between cracks, so that the buckling stress decreases when the distance between

cracks increease. For example, in the case of / 1.5a R = , the buckling stress for / 0.45d L = is 3 times smaller than the case in which / 0.05d L = .

34

Table 3. Critical buckling stresses of an FGM cylindrical shell with three parallel cracks for

various crack lengths and distances between cracks

/a R /d L

0.05 0.125 0.25 0.375 0.45

Critical buckling stress (MPa)

0.7 61.55 57.34 50.75 43.90 38.07

1.0 25.56 24.80 21.11 13.41 10.67

1.2 15.42 11.86 9.31 5.85 4.84

1.5 10.66 7.05 5.28 3.30 2.53

The buckling mode shapes related to / 1 /10 and / 1/ 3d L d L= = and their associated

buckling stresses for the crack length to radius ratio / 1.5a R = and 0.5n = are depicted in Fig. 22. Clearly, the distances between the cracks can crucially alter the buckling behavior of

the shell.

35

Fig. 22. The first four buckling mode shapes of the FGM cylindrical shell for two different

values of /d L , a) / 1/ 3d L = b) / 1/10d L =

36

Conclusion:

A comprehensive study on the buckling behavior of cracked FGM cylindrical shells has been

performed by the extended finite element method to numerically solve the stability equation. First, the method has been verified by the analysis of reference cracked isotropic cylindrical

shells. It has been illustrated that not only the present XFEM formulation is accurate enough,

it is also computationally more efficient than the conventional finite element method. From

the computational cost standpoint, the work presented herein is several times more efficient

compared with, for example, the work done by Seifi et al [43]. Then, the method has been

implemented to analyze the buckling behavior of a cracked FGM cylindrical shell under three

different loading conditions and also an FGM cylindrical shell with three parallel cracks

under axial compression. The effects of several parameters such as crack lengths and angles,

aspect ratios of the shell and the gradient index of the material on the buckling behavior of

the problem have been examined thoroughly.

Some of the most important conclusions of the study can be outlined as follows:

In general, as the length of the crack increases, the critical buckling stress of the shell drops. The same conclusion can be made about the gradient index of the functionally

graded material ( n ). Thus, the value of the critical buckling stress of the FGM

cylindrical shell is highly depends on the aforementioned parameters.

The buckling behavior of the FGM shell is under the severe influence of the angle of the crack ( ). So much so that in tension, as the angle of the crack heightens, the critical buckling stress of the shell noticeably increases, whereas in compression, due

to the complex nature of the mechanics of the problem, a definite conclusion cannot

be made. Nevertheless, for 90 = , the critical buckling stress is minimized.

It is obvious that the thickness of the FGM shell can greatly affect the critical buckling stress of the FGM shell.

The length of the shell, also, plays an important role in the buckling behavior of the FGM shell. As the length of the shell decreases, the buckling stress of the shell experiences a drop. This assertion can be attributed to both tensile and compressive

external loads. But the effect is much more strongly felt in tension.

The effect of the internal pressure on the buckling of shell has been thoroughly

investigated for two different crack angles ( 0 90and = = ). It was observed that

when crack is along the axis of the shell, the increase in the internal pressure of the

FGM shell results in a significant reduction in the buckling stress. For 0 = , the internal pressure in the FGM shell exerts a stabilizing effect on the critical buckling

stress. i.e. as the internal pressure increases, the buckling stress increase as well.

Acknowledgements

The authors wish to gratefully acknowledge the technical support of the High Performance

Computing Lab, School of Civil Engineering, University of Tehran. Also, the first author

would like to extend his gratitude to Dr Hamid Bayesteh for his invaluable contributions

which improved the quality of the present research.

37

References

[1] Ng T, Lam K, Liew K, Reddy J. Dynamic stability analysis of functionally graded cylindrical shells

under periodic axial loading. International Journal of Solids and Structures. 2001;38:1295-309.

[2] Sofiyev A. The stability of compositionally graded ceramicmetal cylindrical shells under aperiodic

axial impulsive loading. Composite structures. 2005;69:247-57.

[3] Bagherizadeh E, Kiani Y, Eslami M. Mechanical buckling of functionally graded material cylindrical

shells surrounded by Pasternak elastic foundation. Composite structures. 2011;93:3063-71.

[4] Huang H, Han Q. Nonlinear dynamic buckling of functionally graded cylindrical shells subjected to

time-dependent axial load. Composite structures. 2010;92:593-8.

[5] Shariyat M. Dynamic thermal buckling of suddenly heated temperature-dependent FGM

cylindrical shells, under combined axial compression and external pressure. International Journal of

Solids and Structures. 2008;45:2598-612.

[6] Shen H-S. Postbuckling analysis of pressure-loaded functionally graded cylindrical shells in

thermal environments. Engineering Structures. 2003;25:487-97.

[7] Shen H-S. Thermal postbuckling behavior of functionally graded cylindrical shells with

temperature-dependent properties. International Journal of Solids and Structures. 2004;41:1961-74.

[8] Shen H-S, Noda N. Postbuckling of FGM cylindrical shells under combined axial and radial

mechanical loads in thermal environments. International Journal of Solids and Structures.

2005;42:4641-62.

[9] Shen H-S, Noda N. Postbuckling of pressure-loaded FGM hybrid cylindrical shells in thermal

environments. Composite structures. 2007;77:546-60.

[10] Wu L, Jiang Z, Liu J. Thermoelastic stability of functionally graded cylindrical shells. Composite

structures. 2005;70:60-8.

[11] Estekanchi H, Vafai A. On the buckling of cylindrical shells with through cracks under axial load.

Thin-walled structures. 1999;35:255-74.

[12] Vafai A, Estekanchi H. A parametric finite element study of cracked plates and shells. Thin-

walled structures. 1999;33:211-29.

[13] Vaziri A, Estekanchi H. Buckling of cracked cylindrical thin shells under combined internal

pressure and axial compression. Thin-walled structures. 2006;44:141-51.

[14] Vaziri A. On the buckling of cracked composite cylindrical shells under axial compression.

Composite structures. 2007;80:152-8.

[15] Javidruzi M, Vafai A, Chen J, Chilton J. Vibration, buckling and dynamic stability of cracked

cylindrical shells. Thin-walled structures. 2004;42:79-99.

[16] Tafreshi A. Efficient modelling of delamination buckling in composite cylindrical shells under

axial compression. Composite structures. 2004;64:511-20.

[17] Tafreshi A. Delamination buckling and postbuckling in composite cylindrical shells under

combined axial compression and external pressure. Composite structures. 2006;72:401-18.

[18] Tafreshi A. Instability of delaminated composite cylindrical shells under combined axial

compression and bending. Composite structures. 2008;82:422-33.

[19] Nasirmanesh A, Mohammadi S. XFEM buckling analysis of cracked composite plates. Composite

structures. 2015;131:333-43.

[20] Natarajan S, Chakraborty S, Ganapathi M, Subramanian M. A parametric study on the buckling

of functionally graded material plates with internal discontinuities using the partition of unity

method. European Journal of Mechanics-A/Solids. 2014;44:136-47.

[21] Liu P, Bui T, Zhu D, Yu T, Wang J, Yin S, et al. Buckling failure analysis of cracked functionally

graded plates by a stabilized discrete shear gap extended 3-node triangular plate element.

Composites Part B: Engineering. 2015;77:179-93.

[22] Baiz P, Natarajan S, Bordas S, Kerfriden P, Rabczuk T. Linear buckling analysis of cracked plates

by SFEM and XFEM. Journal of Mechanics of Materials and Structures. 2012;6:1213-38.

[23] Afshar A, Daneshyar A, Mohammadi S. XFEM analysis of fiber bridging in mixed-mode crack

propagation in composites. Composite structures. 2015;125:314-27.

38

[24] Ardakani SH, Afshar A, Mohammadi S. Numerical study of thermo-mechanical coupling effects

on crack tip fields of mixed-mode fracture in pseudoelastic shape memory alloys. International

Journal of Solids and Structures. 2015.

[25] Ardakani SH, Ahmadian H, Mohammadi S. Thermo-mechanically coupled fracture analysis of

shape memory alloys using the extended finite element method. Smart Materials and Structures.

2015;24:045031.

[26] Asadpoure A, Mohammadi S. Developing new enrichment functions for crack simulation in

orthotropic media by the extended finite element method. International Journal for Numerical

Methods in Engineering. 2007;69:2150-72.

[27] Asadpoure A, Mohammadi S, Vafai A. Crack analysis in orthotropic media using the extended

finite element method. Thin-walled structures. 2006;44:1031-8.

[28] Asadpoure A, Mohammadi S, Vafai A. Modeling crack in orthotropic media using a coupled finite

element and partition of unity methods. Finite Elements in analysis and Design. 2006;42:1165-75.

[29] Belytschko T, Mos N, Usui S, Parimi C. Arbitrary discontinuities in finite elements. International

Journal for Numerical Methods in Engineering. 2001;50:993-1013.

[30] Motamedi D, Mohammadi S. Dynamic crack propagation analysis of orthotropic media by the

extended finite element method. International Journal of Fracture. 2010;161:21-39.

[31] Afshar A, Ardakani SH, Mohammadi S. Transient analysis of stationary interface cracks in

orthotropic bi-materials using oscillatory crack tip enrichments. Composite Structures. 2016.

[32] Ashari S, Mohammadi S. Delamination analysis of composites by new orthotropic bimaterial

extended finite element method. International Journal for Numerical Methods in Engineering.

2011;86:1507-43.

[33] Bayesteh H, Mohammadi S. XFEM fracture analysis of orthotropic functionally graded materials.

Composites Part B: Engineering. 2013;44:8-25.

[34] Rashetnia R, Mohammadi S. Finite strain fracture analysis using the extended finite element

method with new set of enrichment functions. International Journal for Numerical Methods in

Engineering. 2015;102:1316-51.

[35] Nguyen-Thanh N, Valizadeh N, Nguyen M, Nguyen-Xuan H, Zhuang X, Areias P, et al. An

extended isogeometric thin shell analysis based on KirchhoffLove theory. Computer Methods in

Applied Mechanics and Engineering. 2015;284:265-91.

[36] Rabczuk T, Areias P. A meshfree thin shell for arbitrary evolving cracks based on an extrinsic

basis. 2006.

[37] Rabczuk T, Areias P, Belytschko T. A meshfree thin shell method for non-linear dynamic fracture.

International Journal for Numerical Methods in Engineering. 2007;72:524-48.

[38] Amiri F, Milln D, Shen Y, Rabczuk T, Arroyo M. Phase-field modeling of fracture in linear thin

shells. Theoretical and Applied Fracture Mechanics. 2014;69:102-9.

[39] Areias P, Rabczuk T, Msekh M. Phase-field analysis of finite-strain plates and shells including

element subdivision. Computer Methods in Applied Mechanics and Engineering. 2016.

[40] Bayesteh H, Mohammadi S. XFEM fracture analysis of shells: the effect of crack tip enrichments.

Computational Materials Science. 2011;50:2793-813.

[41] Mohammadi S. Extended finite element method: for fracture analysis of structures: John Wiley

& Sons, 2008.

[42] Cook RD. Concepts and applications of finite element analysis: John Wiley & Sons, 2007.

[43] Seifi R, Googarchin HS, Farrokhi M. Buckling of cracked cylindrical panels under axially

compressive and tensile loads. Thin-walled structures. 2015;94:457-65.

[44] Hajlaoui A, Jarraya A, El Bikri K, Dammak F. Buckling Analysis of Functionally Graded Materials

Structures with Enhanced Solid-Shell Elements and Transverse Shear Correction. Composite

Structures. 2015.